ICCES Evaluation Reports are not to be construed as representing aesthetics or any other attributes not specifically addressed, nor are they to be construed
as an endorsement of the subject of the report or a recommendation for its use. There is no warranty by ICC Evaluation Service, LLC, express or implied, as
to any finding or other matter in this report, or as to any product covered by the report.
Copyright © 2013 Page 1 of 5
1000
ICCES Evaluation Report
ESR2107
Issued January 1, 2013
This report is subject to renewal January 1, 2014.
www.icces.org  (800) 4236587  (562) 6990543 A Subsidiary of the International Code Council
®
DIVISION: 03 00 00—CONCRETE
Section: 03 21 00—Reinforcing Steel
REPORT HOLDER:
MMFX STEEL CORPORATION OF AMERICA
2415 CAMPUS DRIVE, SUITE 100
IRVINE, CALIFORNIA 92612
(949) 4767600
www.mmfx.com
info@mmfx.com
EVALUATION SUBJECT:
ASTM A1035/A1035M GRADE 100 STEEL REINFORCING
BARS
1.0 EVALUATION SCOPE
Compliance with the following codes:
2012 and 2009 International Building Code
®
(IBC)
Property evaluated:
Structural
2.0 USES
ASTM A1035/A1035M Grade 100 steel reinforcing bars
are deformed steel reinforcing bars used as longitudinal
and transverse reinforcement in reinforced concrete
structural members, such as foundations, columns and
walls.
3.0 DESCRIPTION
3.1 ASTM A1035/A1035M Grade 100 Bars:
ASTM A1035/A1035M Grade 100 Bars are deformed steel
reinforcing bars available in Nos. 3 to 18 sizes. Examples
of available bars are illustrated in Figure 1. Nominal
weights, dimensions, and deformations comply with values
given in Table 1 of ASTM A1035.
3.2 Materials:
The bars are rolled from identified heats of cast steel and
comply with requirements in ASTM A1035/A1035M for
Grade 100. The specified yield strength is 100,000 psi
(690 MPa) and the specified tensile strength is 150,000 psi
(1030 MPa).
4.0 DESIGN AND INSTALLATION
4.1 Design:
The bars must be designed in accordance with ACI 318
and ACI ITG6R, as summarized in Annex 1 of this report,
entitled, “Design Methodology, ASTM A1035/A1035M
Grade 100 Bars.”
The following limitations also apply:
1. The reinforcing bars must not be used as longitudinal
reinforcement in special moment frame members,
special structural wall boundary elements, or coupling
beams.
2. The ASTM A1035 Grade 100 reinforcing bars must not
be welded.
3. The ASTM A1035 Grade 100 reinforcing bars must not
be used as headed deformed bars in tension.
4. The specified compressive strength for concrete must
range from 4,000 psi to 12,000 psi (27.6 MPa to
82.7 MPa).
5. Use of the ASTM A1035 Grade 100 reinforcing bars is
applicable to reinforcement under Sections 3.5.3.2,
3.5.3.3, 9.4, 11.4.2, 11.5.3.4 11.6.6, 18.9.3.2, and
19.3.2 of ACI 318, which is referenced in Section 1901.2
of the IBC.
6. For structures assigned to Seismic Design Category
(SDC) D, E, or F, ASTM A1035 Grade 100 reinforcing
bars are limited to placement in slab systems,
foundations, and structural components not designated
as part of the seismic force–resisting system but
explicitly analyzed for induced effects of design
displacements in accordance with ACI 318 Section
21.13. Additional requirements pertaining to structures
assigned to SDC D, E, or F are described in Section
A.2.20 of this report.
4.2 Installation:
4.2.1 ASTM A1035/A1035M Grade 100 Bars: The bars
and splices must be located in the structure as set forth in
the approved drawings and specifications. Reinforcement
details, including surface conditions, bar placement, clear
spacing, offsets, spirals and ties, must comply with the
applicable provisions in Chapter 7 of ACI 318
4.2.2 Mechanical Splices: Mechanical splices are
beyond the scope of this report. Mechanical connectors
must be recognized in an ICCES evaluation report and
specifically permitted for use with MMFX ASTM
A1035/A1035M Grade 100 bars.
4.3 Special Inspection:
Special inspection is required in accordance with 2012 IBC
Section 1705.3 or 2009 IBC Section 1704.4. The special
inspector must verify the following:
1. That reinforcing steels are of the type, grade and size
specified and are labeled in conformance with this
report.
ESR2107

Most Widely Accepted and Trusted Page 2 of 5
2. That bending of reinforcing steel bars complies with ACI
31811 Section 7.3 under the 2012 IBC, or with 2009
IBC Section 1907.3, and the modifications given in
Annex 1 Section A2.1.
3. That reinforcing steel surface conditions comply with
ACI 31811 Section 7.4 under the 2012 IBC, or with
2009 IBC Section 1907.4.
4. That reinforcing steels are placed within tolerances set
forth in ACI 31811 Section 7.5 under the 2012 IBC, or
with 2009 IBC Section 1907.5; and are adequately
supported and secured to prevent displacement during
concrete placement.
5. That minimum concrete protection is provided in
accordance with ACI 31811 Section 7.7 under the 2012
IBC, or with 2009 IBC Section 1907.7.
6. That placement of reinforcing steel complies with
required spacing, profile and quantity requirements, as
specified in the approved drawings and specifications.
7. That hooks, bends, ties, stirrups and supplemental
reinforcement are fabricated and placed as specified in
the approved drawings and specifications.
8. That lap lengths, stagger and offsets are provided in
accordance with the approved drawings and
specifications.
5.0 CONDITIONS OF USE
The ASTM A1035/A1035M Grade 100 Bars described in
this report comply with applicable provisions of the codes
indicated in Section 1.0 of this report, subject to the
following conditions:
5.1 The bars must be installed in accordance with the
applicable code, the manufacturer's instructions and
this report. In case of conflict between the
manufacturer's published instructions and this report,
the more restrictive governs.
5.2 Splice locations must comply with applicable code
requirements and be noted on drawings approved by
the building official.
5.3 Prior to installation, calculations and details
demonstrating compliance with this report must be
submitted to the building official. The calculations and
details must be prepared by a registered design
professional where required by the statutes of the
jurisdiction in which the project is to be constructed.
5.4 Use in structures assigned to Seismic Design
Categories D, E, or F and regulated by Chapter 21 of
ACI 318 are beyond the scope of this report, except
as noted in Section 4.1.6 of this report.
5.5 Special inspection must be provided in accordance
with Section 4.3 of this report.
5.6 Limitations listed in Section 4.1 of this report must be
observed.
6.0 EVIDENCE SUBMITTED
Data in accordance with the ICCES Acceptance Criteria
for Highstrength Reinforcing Bars (AC429), dated June
2012.
7.0 IDENTIFICATION
Each bar is identified in accordance with the provisions of
ASTM A1035/A1035M and AC429 Section 2.1.3.1. Figure
2 provides an explanation of each bar mark. The bar
bundles are identified by tags bearing the manufacturer's
name, the report holder's name (MMFX Steel), the grade,
the number of bars in the bundle, the nominal bar
diameter, bar length, heat number, roll number, and the
evaluation report number (ESR2107).
FIGURE 1—EXAMPLES OF AVAILABLE ASTM A1035 GRADE 100 BARS
FIGURE 2—EXPLANATION OF BAR MARKINGS
ESR2107

Most Widely Accepted and Trusted Page 3 of 5
ANNEX 1—DESIGN METHODOLOGY, ASTM A1035/A1035M GRADE 100 BARS
A1.0 Structural design with highstrength reinforcing bars must be in accordance with ACI 318, as modified by ACI ITG6R.
Table A1 provides the highest permissible values of the specified yield strengths for the ASTM A1035/A1035M Grade 100
bars to be used in the design of structural members.
A2.0 ACI ITG6R provides further guidance for using highstrength steel reinforcing bars beyond current ACI 318 limitations.
The design and installation of ASTM A1035/A1035M Grade 100 bars must observe the following modifications to ACI 318,
taken from ACI ITG6R:
A2.1 Deformed Reinforcement: Modify ACI 318 Section 3.5.3.3 to read as follows:
3.5.3.3—Deformed Grade 100 reinforcing bars conforming to ASTM A1035 shall be permitted to be used subject to
the specific modifications to ACI 318 given in this report. Tensile strain,
ε
s
, shall satisfy the following relationship:
ε
s
≤ 0.015.
A2.2 Exposure Categories and Classes: Modify ACI 318 Section 4.2 by adding new Section 4.2.2:
4.2.2—ASTM A1035 Grade 100 bars shall be permitted to be in direct contact with other grades of steel except
where the structure is in an aqueous environment. Aqueous environments include concrete exposure categories
and classes where moisture or water contact is anticipated, as set forth in Section 4.2.1.
A2.3 Bending: Modify ACI 318 Section 7.3 by adding new Section 7.3.3:
7.3.3—Unbending of ASTM A1035 Grade 100 bars is prohibited.
A2.4 Redistribution of Moments: Modify ACI 318 Section 8.4 by adding the following:
Redistribution of moments shall not apply to members containing ASTM A1035 Grade 100 reinforcing bars.
A2.5 Strength Reduction Factor: Modify by ACI 318 Section 9.3.2.2 by replacing the second paragraph with the
following:
For sections reinforced with ASTM A1035 Grade 100 bars in which the net tensile strain in the extreme tension
steel at nominal strength,
ε
t
, is between the limits for compressioncontrolled and tensioncontrolled sections, φ
shall be permitted to be linearly increased from that for compressioncontrolled sections to 0.90 as
ε
t
increases from
the compressioncontrolled strain limit to 0.009 in accordance with Eq. A21:
φ = 0.45 + 50
ε
t
(Eq. A21)
A2.6 Design Strength for Reinforcement: Modify ACI 318 Section 9.4 to read as follows:
9.4—The specified yield strengths of ASTM A1035 Grade 100 bars used in the design of structural members shall
be no more than the values shown in Table A1.
TABLE A1—SPECIFIED YIELD STRENGTHS FOR DESIGN OF MEMBERS USING ASTM A1035/A1035M
GRADE 100 REINFORCEMENT
1
TYPE OF MEMBER
LONGITUDINAL REINFORCEMENT TRANSVERSE REINFORCEMENT
Tension, psi
(MPa)
Compression, psi
(MPa)
Shear, psi
(MPa)
Torsion, psi
(MPa)
Confinement, psi
(MPa)
Beams and oneway slabs 100,000 (690) 80,000 (550) 80,000 (550) 60,000 (410) N/A
Columns 100,000 (690) 80,000 (550) 80,000 (550) 60,000 (410) 100,000 (690)
2
Tension ties 80,000 (550) N/A N/A N/A N/A
Compression struts N/A 80,000 (550) N/A N/A N/A
Twoway slabs 100,000 (690) 80,000 (550) 60,000 (410) 60,000 (410) N/A
Walls 100,000 (690) 80,000 (550) 80,000 (550) N/A 100,000 (690)
3
Footings and pile caps 100,000 (690) 80,000 (550) 80,000 (550) 60,000 (410) N/A
Mat foundations 100,000 (690) 80,000 (550) 80,000 (550) N/A N/A
1
N/A = Not applicable
2
Spirals and ties
3
Ties
A2.7 Control of Deflections: Modify ACI 318 Table 9.5(a) by adding the following note:
c) This table does not apply to members reinforced with ASTM A1035 Grade 100 bars. Deflections shall be computed in
accordance with Section 9.5.2.3.
Replace ACI 318 Eq. (98) with Eq. A22.
I
e =
ூ
ଵି൬ଵି
൰ቀ
ಾ
ಾ
ೌ
ቁ
≤
I
g
(Eq. A22)
ESR2107

Most Widely Accepted and Trusted Page 4 of 5
A2.8 Tensile stress: Modify ACI 318 Section 10.2.4 to read as follows:
10.2.4—Tensile stress in ASTM A1035 Grade 100 bars shall be computed in accordance with Eq. A23 or A24:
f
s
= 29,000
ε
s
(ksi) for
ε
s
≤ 0.0034 (Eq. A23)
100 ksi for 0.0034 <
ε
s
≤ 0.015 (Eq. A24)
A2.9 Compressioncontrolled Strain Limit: Modify ACI 318 Section 10.3.3 to read as follows:
10.3.3—Sections are compressioncontrolled if the net tensile strain in the extreme tension steel,
ε
t
,
is equal to or less
than the compressioncontrolled strain limit when the concrete in compression reaches its assumed strain limit of 0.003.
The compressioncontrolled strain limit is the net tensile strain in the reinforcement at balanced strain conditions. For
ASTM A1035 Grade 100 reinforcement, it shall be permitted to set the compressioncontrolled strain limit equal to 0.004.
A2.10 Tensioncontrolled Strain Limit: Modify ACI 318 Section 10.3.4 to read as follows:
10.3.4—Sections reinforced with ASTM A1035 Grade 100 bars are tensioncontrolled if the net tensile strain in the
extreme tension steel, ε
t,
is equal to or greater than 0.009 when the concrete in compression reaches its assumed strain
limit of 0.003. Sections with ε
t
between the compressioncontrolled strain limit and 0.009 constitute a transition region
between compressioncontrolled and tensioncontrolled sections.
A2.11 Volumetric Spiral Reinforcement Ratio: Modify ACI 318 Section 10.9.3 to read as follows:
10.9.3—Volumetric spiral reinforcement ratio, ρ
s
, shall be not less than the value given by Eq. A25:
ρ
s =
0.45
ቀ
−1ቁ
ᇱ
(
Eq. A25)
where the value of f
yt
used in Eq. (45) shall not exceed 100,000 psi (690 MPa). For f
yt
greater than 60,000 psi (410 MPa)
and ASTM A1035 Grade 100 reinforcement, lap splices according to 7.10.4.5(a) shall not be used.
A2.12 Slenderness Effects: Modify ACI 318 Section 10.10.2 to read as follows:
10.10.2—When slenderness effects are not neglected as permitted by 10.10.1, the design of compression members,
restraining beams, and other supporting members reinforced with ASTM A1035 Grade 100 bars shall be based on the
factored forces and moments from a secondorder analysis satisfying 10.10.5. These members shall also satisfy
10.10.2.1 and 10.10.2.2. The dimensions of each member cross section used in the analysis shall be within 10 percent of
the dimensions of the members shown on the contract documents or the analysis shall be repeated.
A2.13 Shear Strength Provided by Concrete for Nonprestressed Members: Modify ACI 318 Section 11.2.1.1 by adding
the following:
For oneway slabs reinforced with ASTM A1035 Grade 100 bars where (1) ρ is less than one percent; (2) no significant
axial load is present; and (3) no shear reinforcement is provided, V
c
shall be computed in accordance with Eq. A26 or
Eq. A26M:
V
c
=
ଷ
ଷଽାଶ.ଵௗ
ඥ݂
ᇱ
ܾ
௪
݀
(
Eq. A26)
V
c
=
ଵହସ
ଵାଶ.ଵௗ
ඥ
݂
ᇱ
ܾ
௪
݀
(
Eq. A26M)
A2.14 Shear Reinforcement Design Strength: Modify ACI 318 Section 11.4.2 to read as follows:
11.4.2—The values of f
y
and f
yt
used in design of shear reinforcement shall not exceed 60,000 psi (410 MPa), except the
value may be increased to 80,000 psi (550 MPa) for beams and walls where appearance and serviceability due to shear
cracking are not critical design considerations.
A2.15 Minimum Shear Reinforcement: Modify ACI Section 11.4.6.1 by replacing the first paragraph with the following:
A minimum area of shear reinforcement, A
v,min
, shall be provided in all concrete flexural members reinforced with ASTM
A1035 Grade 100 bars where V
u
exceeds 0.5 φ V
c,
except in members satisfying one or more of (a) through (f):
A2.16 Development of Deformed Bars in Tension: Modify ACI 318 Section 12.2 by deleting Sections 12.2.2 and 12.2.3,
renumbering Section 12.2.4 to become 12.2.3 and replacing Section 12.2.2 with the following:
12.2.2—For ASTM A1035 Grade 100 deformed bars, l
d
shall be in accordance with Eq. A27 or Eq. A2.7M:
l
d
=
൬
ᇲ
¼
ି∅ ଶସ ఠ൰ఈ ఉ
ఒ
∅ ଷ. ൬
್
ഘశ ಼
್
൰
d
b
(in.) (Eq. A27)
ESR2107

Most Widely Accepted and Trusted Page 5 of 5
where:
ϕ = 0.8
α = 1.3 for top cast bars
β
c
= 1.0 for uncoated bars
λ = 1.0 for normalweight concrete
K
tr
= (0.52t
r
t
d
A
tr
/sn)ඥ ݂’
(in.) (Eq. A28)
t
r
= 9.6R
r
+ 0.28 ≤ 1.72 (Eq. A29)
t
d
= 0.78d
b
+ 0.22 (in.) (Eq. A210)
ቀ
್ ഘశ ಼
ௗ
್
ቁ ≤ 4.0 (Eq. A211)
In SI units
l
d
=
൬
ᇲ
¼
ି∅ ହ.ସ ఠ൰ఈ ఉ
ఒ
∅ ଵ.଼ଷ
൬
್ ഘశ ಼
್
൰
d
b
(mm) (Eq. A27M)
K
tr
= (6.26t
r
t
d
A
tr
/sn) ඥ ݂’
(mm) (Eq. A28M)
t
r
= 9.6R
r
+ 0.28 ≤ 1.72 (Eq. A29M)
t
d
= 0.03d
b
+ 0.22 (in.) (Eq. A210M)
ቀ
್ ഘశ ಼
ௗ
್
ቁ ≤ 4.0 (Eq. A211M)
A2.17 Development of Deformed Bars in Compression: Modify ACI 318 Section 12.3 by adding the following:
The specified yield strength f
y
in compression of ASTM A1035 Grade 100 bars is limited to 80,000 psi (550 MPa)
maximum.
A2.18 Mechanical and Welded Splices: Modify ACI Section 12.14.3.1 to read as follows:
12.14.3.1—Mechanical splices shall be permitted when specifically recognized for use with ASTM A1035 Grade 100
reinforcing bars in an ICCES evaluation report. Welding of bars is prohibited.
A2.19 Modification of Moments for Twoway Slab Systems: Modify ACI 318 Section 13.6.7 to read as follows:
13.6.7—Modification of negative and positive factored moments using moment redistribution is prohibited in twoway
slabs reinforced with ASTM A1035 Grade 100 bars.
A2.20 Use in Earthquakeresistant structures: Modify ACI Section 21.1.5 by adding new section 21.1.5.6 as follows:
21.1.5.6—Use of ASTM A1035 Grade 100 reinforcing bars as longitudinal reinforcement in a structural member that is
part of the seismicforceresisting system of a building assigned to SDC D, E or F is prohibited. The use of ASTM A1035
Grade 100 reinforcing bars as transverse reinforcement is permitted, provided f
yt
is limited to 60,000 psi (410 MPa)
maximum for computing shear strength.
Modify ACI Section 21.3.2 to read as follows:
21.3.2—Where Grade 60 (420 MPa) reinforcing bars are used for column longitudinal reinforcement and ASTM A1035
Grade 100 reinforcing bars are used for beam longitudinal reinforcement in intermediate moment frames, the flexural
strength requirements (strongcolumnweak beam) in Section 21.6.2.2 shall be met using the actual strengths of the
beams containing ASTM A1035 Grade 100 reinforcement. A nonlinear analysis shall be conducted to determine M
nb
.
The required shear strength of the beam shall be determined based on M
nb
from such nonlinear analysis. Permitted
methods of nonlinear analysis are given in ACI ITG6R.
Σχόλια 0
Συνδεθείτε για να κοινοποιήσετε σχόλιο